This article needs additional citations for "verification. (June 2008) ("Learn how and when to remove this template message)
Paint is any "liquid, liquefiable, or mastic composition that, after application to a "substrate in a thin layer, converts to a "solid film. It is most commonly used to protect, color, or provide texture to objects. Paint can be made or purchased in many colors—and in many different types, such as watercolor, synthetic, etc. Paint is typically stored, sold, and applied as a liquid, but most types dry into a solid.
In 2001 and 2004, South African archeologists reported finds in Blombos Cave of a 100,000-year-old human-made "ochre-based mixture that could have been used like paint. Further excavation in the same cave resulted in the 2011 report of a complete toolkit for grinding pigments and making a primitive paint-like substance. "Cave paintings drawn with red or yellow ochre, "hematite, "manganese oxide, and "charcoal may have been made by early "Homo sapiens as long as 40,000 years ago.
Ancient colored walls at "Dendera, "Egypt, which were exposed for years to the elements, still possess their brilliant color, as vivid as when they were painted about 2,000 years ago. The Egyptians mixed their colors with a gummy substance, and applied them separately from each other without any blending or mixture. They appear to have used six colors: white, black, blue, red, yellow, and green. They first covered the area entirely with white, then traced the design in black, leaving out the lights of the ground color. They used "minium for red, and generally of a dark tinge.
"Pliny mentions some painted ceilings in his day in the town of "Ardea, which had been done prior to the foundation of "Rome. He expresses great surprise and admiration at their freshness, after the lapse of so many centuries.
Paint was made with the yolk of "eggs and therefore, the substance would harden and adhere to the surface it was applied to. Pigment was made from plants, sand, and different soils. Most paints used either oil or water as a "base (the diluent, solvent or vehicle for the pigment).
A still extant example of 17th-century house oil painting is "Ham House in "Surrey, "England, where a primer was used along with several undercoats and an elaborate decorative overcoat; the pigment and oil mixture would have been ground into a paste with a mortar and pestle. The process was done by hand by the painters and exposed them to lead poisoning due to the white-lead powder.
In 1718, Marshall Smith invented a "Machine or Engine for the Grinding of Colours" in England. It is not known precisely how it operated, but it was a device that increased the efficiency of pigment grinding dramatically. Soon, a company called Emerton and Manby was advertising exceptionally low-priced paints that had been ground with labour-saving technology:
By the proper onset of the "Industrial Revolution, paint was being ground in steam-powered mills and an alternative to lead-based pigments was found in a white derivative of zinc oxide. Interior house painting increasingly became the norm as the 19th century progressed, both for decorative reasons and because the paint was effective in preventing the walls rotting from damp. Linseed oil was also increasingly used as an inexpensive binder.
It was not until the stimulus of "World War II created a shortage of linseed oil in the supply market that artificial resins, or alkyds, were invented. Cheap and easy to make, they also held the color well and lasted for a long time.["not in citation given]["citation needed]
The vehicle is composed of the binder; or, if it is necessary to thin the binder with a diluent like solvent or water, it is the combination of binder and diluent. In this case, once the paint has dried or cured very nearly all of the diluent has evaporated and only the binder is left on the coated surface. Thus, an important quantity in coatings formulation is the "vehicle solids", sometimes called the "resin solids" of the formula. This is the proportion of the wet coating weight that is binder, i.e. the polymer backbone of the film that will remain after drying or curing is complete.
The binder is the film-forming component of paint. It is the only component that is always present among all the various types of formulations. Many binders are too thick to be applied and must be thinned. The type of thinner, if present, varies with the binder.
The binder imparts properties such as gloss, durability, flexibility, and toughness.
Binders include synthetic or natural resins such as alkyds, "acrylics, vinyl-acrylics, vinyl acetate/ethylene (VAE), "polyurethanes, "polyesters, "melamine resins, "epoxy, silanes or siloxanes or "oils.
Binders can be categorized according to the mechanisms for film formation. Thermoplastic mechanisms include drying and coalescence. Drying refers to simple evaporation of the solvent or thinner to leave a coherent film behind. Coalescence refers to a mechanism that involves drying followed by actual interpenetration and fusion of formerly discrete particles. Thermoplastic film-forming mechanisms are sometimes described as "thermoplastic cure" but that is a misnomer because no chemical curing reactions are required to knit the film. Thermosetting mechanisms, on the other hand, are true curing mechanism that involve chemical reaction(s) among the polymers that make up the binder.
Thermoplastic mechanisms: Some films are formed by simple cooling of the binder. For example, "encaustic or "wax paints are liquid when warm, and harden upon cooling. In many cases, they resoften or liquify if reheated.
Paints that dry by solvent evaporation and contain the solid binder dissolved in a solvent are known as lacquers. A solid film forms when the solvent evaporates. Because no chemical crosslinking is involved, the film can re-dissolve in solvent; as such, lacquers are unsuitable for applications where chemical resistance is important. Classic "nitrocellulose lacquers fall into this category, as do non-grain raising stains composed of "dyes dissolved in solvent. Performance varies by formulation, but lacquers generally tend to have better "UV resistance and lower corrosion resistance than comparable systems that cure by polymerization or coalescence.
The paint type known as "Emulsion in the UK and "Latex in the United States is a water-borne dispersion of sub-micrometer polymer particles. These terms in their respective countries cover all paints that use synthetic polymers such as acrylic, vinyl acrylic ("PVA), styrene acrylic, etc. as binders. The term "latex" in the context of paint in the United States simply means an aqueous dispersion; "latex rubber from the rubber tree is not an ingredient. These dispersions are prepared by "emulsion polymerization. Such paints cure by a process called coalescence where first the water, and then the trace, or coalescing, solvent, evaporate and draw together and soften the binder particles and fuse them together into irreversibly bound networked structures, so that the paint cannot redissolve in the solvent/water that originally carried it. The residual "surfactants in paint, as well as "hydrolytic effects with some polymers cause the paint to remain susceptible to softening and, over time, degradation by water. The general term of latex paint is usually used in the United States, while the term emulsion paint is used for the same products in the UK and the term latex paint is not used at all.
Thermosetting mechanisms: Paints that cure by polymerization are generally one- or two-package coatings that polymerize by way of a chemical reaction, and cure into a crosslinked film. Depending on composition they may need to dry first, by evaporation of solvent. Classic two-package "epoxies or "polyurethanes would fall into this category.
The "drying oils", counter-intuitively, actually cure by a crosslinking reaction even if they are not put through an oven cycle and seem to simply dry in air. The film formation mechanism of the simplest examples involve first evaporation of solvents followed by reaction with oxygen from the environment over a period of days, weeks and even months to create a crosslinked network. Classic "alkyd enamels would fall into this category. Oxidative cure coatings are catalyzed by metal complex driers such as "cobalt naphthenate.
Recent environmental requirements restrict the use of "volatile organic compounds (VOCs), and alternative means of curing have been developed, generally for industrial purposes. "UV curing paints, for example, enable formulation with very low amounts of solvent, or even none at all. This can be achieved because of the monomers and oligomers used in the coating have relatively very low molecular weight, and are therefore low enough in viscosity to enable good fluid flow without the need for additional thinner. If solvent is present in significant amounts, generally it is mostly evaporated first and then crosslinking is initiated by ultraviolet light. Similarly, "powder coatings contain little or no solvent. Flow and cure are produced by heating of the substrate after electrostatic application of the dry powder.
Combination mechanisms: So-called "catalyzed" lacquers" or "crosslinking latex" coatings are designed to form films by a combination of methods: classic drying plus a curing reaction that benefits from the catalyst. There are paints called plastisols/organosols, which are made by blending PVC granules with a plasticiser. These are stoved and the mix coalesces.
The main purposes of the diluent are to dissolve the polymer and adjust the "viscosity of the paint. It is volatile and does not become part of the paint film. It also controls flow and application properties, and in some cases can affect the stability of the paint while in liquid state. Its main function is as the carrier for the non volatile components. To spread heavier oils (for example, linseed) as in oil-based interior house paint, a thinner oil is required. These volatile substances impart their properties temporarily—once the solvent has evaporated, the remaining paint is fixed to the surface.
This component is optional: some paints have no "diluent.
Water is the main diluent for water-borne paints, even the co-solvent types.
Solvent-borne, also called oil-based, paints can have various combinations of organic solvents as the diluent, including "aliphatics, "aromatics, "alcohols, "ketones and "white spirit. Specific examples are organic solvents such as "petroleum distillate, "esters, "glycol ethers, and the like. Sometimes volatile low-molecular weight synthetic resins also serve as diluents.
Pigments are granular solids incorporated in the paint to contribute color. Fillers are granular solids incorporate to impart toughness, texture, give the paint special properties, or to reduce the cost of the paint. Alternatively, some paints contain "dyes instead of or in combination with pigments.
Pigments can be classified as either natural or synthetic. Natural pigments include various "clays, "calcium carbonate, "mica, "silicas, and "talcs. Synthetics would include engineered molecules, "calcined clays, "blanc fixe, precipitated calcium carbonate, and synthetic pyrogenic silicas.
Hiding pigments, in making paint opaque, also protect the substrate from the harmful effects of "ultraviolet light. Hiding pigments include "titanium dioxide, "phthalo blue, "red iron oxide, and many others.
Fillers are a special type of pigment that serve to thicken the film, support its structure and increase the volume of the paint. Fillers are usually cheap and inert materials, such as "diatomaceous earth, "talc, "lime, "barytes, clay, etc. Floor paints that must resist abrasion may contain fine quartz sand as a filler. Not all paints include fillers. On the other hand, some paints contain large proportions of pigment/filler and binder.
Some pigments are toxic, such as the "lead pigments that are used in "lead paint. Paint manufacturers began replacing white lead pigments with titanium white (titanium dioxide), before lead was banned in paint for residential use in 1978 by the US Consumer Product Safety Commission. The titanium dioxide used in most paints today is often coated with silica/alumina/zirconium for various reasons, such as better exterior durability, or better hiding performance (opacity) promoted by more optimal spacing within the paint film.
Micaceous "iron oxide (MIO) is another alternative to lead for protection of steel, giving more protection against water and light damage than most paints. When MIO pigments are ground into fine particles, most cleave into shiny layers, which reflect light, thus minimising "UV degradation and protecting the "resin binder. Most pigments used in paint tend to be spherical, but lamellar pigments, such as glass flake and MIO have overlapping plates, which impede the path of water molecules. For optimum performance MIO should have a high content of thin flake-like particles resembling "mica. "ISO 10601 sets two levels of MIO content. MIO is often derived from a form of "hematite.
Besides the three main categories of ingredients, paint can have a wide variety of miscellaneous additives, which are usually added in small amounts, yet provide a significant effect on the product. Some examples include additives to modify "surface tension, improve flow properties, improve the finished appearance, increase wet edge, improve pigment stability, impart "antifreeze properties, control foaming, control skinning, etc. Other types of additives include "catalysts, thickeners, stabilizers, "emulsifiers, texturizers, adhesion promoters, UV stabilizers, flatteners (de-glossing agents), biocides to fight "bacterial growth, and the like.
Additives normally do not significantly alter the percentages of individual components in a formulation.
Various technologies exist for making paints that change color. Thermochromic paints and coatings contain materials that change conformation when heat is applied or removed, and so they change color. "Liquid crystals have been used in such paints, such as in the thermometer strips and tapes used in aquaria and novelty/promotional thermal cups and straws. These materials are used to make eyeglasses.
Color-changing paints can also be made by adding halochrome compounds or other organic pigments. One patent cites use of these indicators for wall coating applications for light colored paints. When the paint is wet it is pink in color but upon drying it regains its original white color. As cited in patent, this property of the paint enabled two or more coats to be applied on a wall properly and evenly. The previous coats having dried would be white whereas the new wet coat would be distinctly pink. Ashland Inc. introduced foundry refractory coatings with similar principle in 2005 for use in foundries.
Electrochromic paints change color in response to an applied electric current. Car manufacturer "Nissan has been reportedly working on an electrochromic paint, based on particles of "paramagnetic "iron oxide. When subjected to an electromagnetic field the paramagnetic particles change spacing, modifying their color and reflective properties. The electromagnetic field would be formed using the conductive metal of the car body. Electrochromic paints can be applied to plastic substrates as well, using a different coating chemistry. The technology involves using special dyes that change conformation when an electric current is applied across the film itself. This new technology has been used to achieve glare protection at the touch of a button in passenger airplane windows.
Since the time of the "Renaissance, "siccative "(drying) oil paints, primarily "linseed oil, have been the most commonly used kind of paints in fine art applications; "oil paint is still common today. However, in the 20th century, water-based paints, including "watercolors and "acrylic paints, became very popular with the development of "acrylic and other latex paints. "Milk paints (also called "casein), where the medium is derived from the natural emulsion that is "milk, were popular in the 19th century and are still available today. "Egg tempera (where the medium is an "emulsion of raw "egg yolk mixed with oil) is still in use as well, as are encaustic "wax-based paints. "Gouache is a variety of opaque watercolor that was also used in the "Middle Ages and Renaissance for manuscript illuminations. The pigment was often made from ground semiprecious stones such as "lapis lazuli and the binder made from either "gum arabic or "egg white. Gouache, also known as 'designer color' or 'body color' is commercially available today.
"Poster paint has been used primarily in the creation of student works, or by children.
Paint can be applied as a solid, a gaseous suspension ("aerosol) or a liquid. Techniques vary depending on the practical or artistic results desired.
As a solid (usually used in industrial and automotive applications), the paint is applied as a very fine powder, then baked at high temperature. This melts the powder and causes it to adhere to the surface. The reasons for doing this involve the chemistries of the paint, the surface itself, and perhaps even the chemistry of the substrate (the object being painted). This is called ""powder coating" an object.
As a gas or as a gaseous suspension, the paint is suspended in solid or liquid form in a gas that is "sprayed on an object. The paint sticks to the object. This is called "spray painting" an object. The reasons for doing this include:
Rollers generally have a handle that allows for different lengths of poles to be attached, allowing painting at different heights. Generally, roller application requires two coats for even color. A roller with a thicker "nap is used to apply paint on uneven surfaces. Edges are often finished with an angled brush.
After liquid paint is applied, there is an interval during which it can be blended with additional painted regions (at the "wet edge") called "open time". The open time of an oil or alkyd-based emulsion paint can be extended by adding "white spirit, similar glycols such as Dowanol (propylene glycol ether) or open time prolongers. This can also facilitate the mixing of different wet paint layers for aesthetic effect. Latex and acrylic emulsions require the use of drying retardants suitable for water-based coatings.
Paint application by spray is the most popular method in industry. In this, paint is atomized by the force of compressed air or by the action of high pressure compression of the paint itself, and the paint is turned into small droplets that travel to the article to be painted. Alternate methods are airless spray, hot spray, hot airless spray, and any of these with an electrostatic spray included. There are numerous electrostatic methods available.
Dipping used to be the norm for objects such as filing cabinets, but this has been replaced by high speed air turbine driven bells with electrostatic spray. Car bodies are primed using cathodic elephoretic primer, which is applied by charging the body depositing a layer of primer. The unchanged residue is rinsed off and the primer stoved.
Many paints tend to separate when stored, the heavier components settling to the bottom, and require mixing before use. Some paint outlets have machines for mixing the paint by shaking the can vigorously for a few minutes.
The opacity and the film thickness of paint may be measured using a "drawdown card.
Water-based paints tend to be the easiest to clean up after use; the brushes and rollers can be cleaned with soap and water.
Proper disposal of left over paint is a challenge. Sometimes it can be recycled: Old paint may be usable for a primer coat or an intermediate coat, and paints of similar chemistry can be mixed to make a larger amount of a uniform color.
To dispose of paint it can be dried and disposed of in the domestic waste stream, provided that it contains no prohibited substances (see container). Disposal of liquid paint usually requires special handling and should be treated as hazardous waste, and disposed of according to local regulations.
The main reasons of paint failure after application on surface are the applicator and improper treatment of surface.
Defects or degradation can be attributed to:
"Volatile organic compounds (VOCs) in paint are considered harmful to the environment and especially for people who work with them on a regular basis. Exposure to VOCs has been related to "organic solvent syndrome, although this relation has been somewhat controversial. The controversial solvent "2-butoxyethanol is also used in paint production.
In the US, environmental regulations, consumer demand, and advances in technology led to the development of low-VOC and zero-VOC paints and finishes. These new paints are widely available and meet or exceed the old high-VOC products in performance and cost-effectiveness while having significantly less impact on human and environmental health.["citation needed]
A polychlorinated biphenyl (PCB) was reported ( published in 2009 ) in air samples collected in Chicago, Philadelphia, the Arctic, and several sites around the Great Lakes. PCB is a global pollutant and was measured in the wastewater effluent from paint production. The widespread distribution of PCB suggests volatilization of this compound from surfaces, roofs etc. PCB is present in consumer goods including newspapers, magazines, and cardboard boxes, which usually contain color pigments. Therefore, exist hypothesis that PCB congeners are present as byproduct in some current commercial pigments.
Work published in 2001 described 28 bone tools and thousands of pieces of ocher—a mineral used to create paint for body decoration and cave painting—dated at roughly 70,000 years old found in Blombos Cave in South Africa. Two pieces of ocher appear to be marked with abstract lines that could be viewed as artistic expression.
|Look up paint in Wiktionary, the free dictionary.|
|Wikimedia Commons has media related to paint.|